DOI: 10.17188/1283913
title: Materials Data on LiNbP4O13 by Materials Project

description: LiNbP4O13 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are four inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a trigonal planar geometry to three O2- atoms. There are a spread of Li–O bond distances ranging from 1.86–1.90 Å. In the second Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.93–2.60 Å. In the third Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.93–2.59 Å. In the fourth Li1+ site, Li1+ is bonded in a trigonal planar geometry to three O2- atoms. There is two shorter (1.87 Å) and one longer (1.88 Å) Li–O bond length. There are four inequivalent Nb5+ sites. In the first Nb5+ site, Nb5+ is bonded to six O2- atoms to form NbO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Nb–O bond distances ranging from 1.98–2.04 Å. In the second Nb5+ site, Nb5+ is bonded to six O2- atoms to form NbO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Nb–O bond distances ranging from 1.97–2.04 Å. In the third Nb5+ site, Nb5+ is bonded to six O2- atoms to form NbO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Nb–O bond distances ranging from 1.98–2.03 Å. In the fourth Nb5+ site, Nb5+ is bonded to six O2- atoms to form NbO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Nb–O bond distances ranging from 1.97–2.03 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 43°. There are a spread of P–O bond distances ranging from 1.47–1.60 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–38°. There are a spread of P–O bond distances ranging from 1.46–1.67 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 46°. There are a spread of P–O bond distances ranging from 1.47–1.62 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 43°. There are a spread of P–O bond distances ranging from 1.47–1.61 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 38°. There are a spread of P–O bond distances ranging from 1.48–1.63 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–39°. There are a spread of P–O bond distances ranging from 1.46–1.67 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 44°. There are a spread of P–O bond distances ranging from 1.47–1.62 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 41°. There are a spread of P–O bond distances ranging from 1.47–1.60 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–37°. There are a spread of P–O bond distances ranging from 1.46–1.64 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–38°. There are a spread of P–O bond distances ranging from 1.46–1.64 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–39°. There are a spread of P–O bond distances ranging from 1.48–1.63 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 45°. There are a spread of P–O bond distances ranging from 1.47–1.61 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 42°. There are a spread of P–O bond distances ranging from 1.47–1.60 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–37°. There are a spread of P–O bond distances ranging from 1.48–1.66 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one NbO6 octahedra and corners with two PO4 tetrahedra. The corner-sharing octahedral tilt angles are 40°. There are a spread of P–O bond distances ranging from 1.47–1.60 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two NbO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–37°. There are a spread of P–O bond distances ranging from 1.47–1.66 Å. There are fifty-two inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the second O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the third O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the twelfth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the fourteenth O2- site, O2- is bonded in a distorted water-like geometry to one Li1+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the sixteenth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one Nb5+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the twenty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the twenty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the thirty-first O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the thirty-second O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted water-like geometry to one Li1+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the fortieth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the forty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the forty-second O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the forty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the forty-fourth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the forty-fifth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the forty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the forty-seventh O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the forty-eighth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the forty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the fiftieth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Nb5+, and one P5+ atom. In the fifty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom. In the fifty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one Nb5+ and one P5+ atom.